psi$ and $t$ are the singlet and triplet order parameters respectively. For a range of values of $\nu=\psi/t$, $\Delta_{-}(\mathbf{k})$ can change sign and nodes may exist in the superconducting gap.

Recent band structure calculations for these compounds [@Lee; @2005] provide information about $\mid\mathbf{g(k)}\mid$. These results indicate that $\alpha$ is a large energy scale relative to the bandwidth and that $%
\mid\mathbf{g(k)}\mid$ is highly anisotropic. To capture these results in a model we take:$\mathbf{g(k)}=a_1\mathbf{k}-a_2[\widehat{\mathbf{x}}k_x(k_y2+k_z2)+%
\widehat{\mathbf{y}}k_y(k_z2+k_x2)+\widehat{\mathbf{z}}k_z(k_x2+k_y2)]$,with $a_2/a_1=3/2$, $\mathbf{k}$, a unit vector, and the spherical average of $\mid\mathbf{g(k)}\mid^2$ equal to unity. This form of $\mid\mathbf{g(k)}%
\mid$ is the simplest that is consistent with cubic symmetry and allows for anisotropy on a model, spherical Fermi surface.

![(Color online). The temperature dependence of (a) the normalized penetration depth $\protect\lambda(T)/\protect\lambda_0$ and (b) the corresponding superfluid density $\protect\rho_s(T)$ for Li$_2$Pd$_3$B, in which $T_c=7$ K, $G=0.42$ nm/Hz for sample \#1 and $T_c=6.7$ K, $G=0.63$ nm/Hz for sample \#2. The symbols, as described in the figure, represent the experimental data and the solid line is a theoretical fit with parameters $%
\protect\delta=0.1$ and $\protect\nu=4$. The insets in the upper panel and the lower panel show a 3-dimensional (3D) polar plot of the gap function $%
\Delta_{-}(\mathbf{k})$, and the temperature dependence of the order parameter components $\protect\psi$ (spin singlet) and $t$ (spin triplet), respectively. ](Fig2.eps){
psi$ and $ t$ are the singlet and triplet order parameters respectively. For a range of value of $ \nu=\psi / t$, $ \Delta_{-}(\mathbf{k})$ can transfer sign and nodes may exist in the superconducting gap. 

 late band structure calculations for these compound [ @Lee; @2005 ] provide information about $ \mid\mathbf{g(k)}\mid$. These consequence indicate that $ \alpha$ is a large department of energy scale relative to the bandwidth and that $% 
 \mid\mathbf{g(k)}\mid$ is highly anisotropic. To capture these results in a exemplar we take:$\mathbf{g(k)}=a_1\mathbf{k}-a_2[\widehat{\mathbf{x}}k_x(k_y2+k_z2)+% 
 \widehat{\mathbf{y}}k_y(k_z2+k_x2)+\widehat{\mathbf{z}}k_z(k_x2+k_y2)]$,with $ a_2 / a_1=3/2 $, $ \mathbf{k}$, a unit vector, and the spherical average of $ \mid\mathbf{g(k)}\mid^2 $ equal to unity. This form of $ \mid\mathbf{g(k)}% 
 \mid$ is the simple that is consistent with cubic symmetry and allows for anisotropy on a mannequin, spherical Fermi surface. 

! [ (Color online). The temperature dependence of (a) the normalized penetration depth $ \protect\lambda(T)/\protect\lambda_0 $ and (b) the match superfluid density $ \protect\rho_s(T)$ for Li$_2$Pd$_3$B, in which $ T_c=7 $ K, $ G=0.42 $ nm / Hz for sample \#1 and $ T_c=6.7 $ K, $ G=0.63 $ nm / Hz for sample distribution \#2. The symbols, as described in the figure, represent the experimental data and the solid lineage is a theoretical fit with parameters $% 
 \protect\delta=0.1 $ and $ \protect\nu=4$. The insets in the upper panel and the lower panel show a 3 - dimensional (3D) polar plot of the gap affair $% 
 \Delta_{-}(\mathbf{k})$, and the temperature dependence of the order argument component $ \protect\psi$ (tailspin singlet) and $ t$ (spin triplet), respectively. ] (Fig2.eps) {
psi$ and $t$ are the singlet akd triplet order paramevers reapectiveuy. For a range of values of $\iu=\psu/t$, $\Deota_{-}(\mathbf{k})$ can change rign and jodes mat exmst in the superrknductiky gap.

Dccent uand structure galculationv for these cokpuuuds [@Lee; @2005] provide information about $\myd\mathbg{g(n)}\mid$. These resolts pnqicafv uhat $\alpha$ is a large energy scals relatpve to the bandwicth and that $%
\mid\mathbf{g(k)}\mif$ is highly anisotropif. To capturg thqwe results iv a model we take:$\mathbr{g(k)}=a_1\mathbf{k}-a_2[\widehat{\mathbf{x}}k_x(k_y2+k_x2)+%
\widekat{\mathbf{y}}k_i(k_a2+k_d2)+\fidehat{\mathuf{z}}k_z(k_q2+k_y2)]$,with $a_2/a_1=3/2$, $\mabnbf{k}$, a unit vrctor, and the xphxricql average of $\mid\mathuf{g(k)}\mid^2$ equal to unijy. This fosm of $\mid\mathbf{g(k)}%
\mie$ us thg sim[lesg thxt js cknsistfnt with cubid symmetry qnd allows for anisptwipy on a modem, sphewisal Fermi surface.

![(Color online). The tempegatude dependence of (a) the bormalized penetratioj depth $\pwotect\lambda(T)/\protect\lambda_0$ and (b) the correspondinc supxrwlune denrutj $\protect\rho_s(T)$ for Li$_2$Pd$_3$B, in which $T_c=7$ K, $G=0.42$ nm/Hz rot xample \#1 and $T_c=6.7$ K, $G=0.63$ nm/Hz fpr ssiple \#2. The symcols, as dsscribed in the fihure, rekresenr the exptrimemtal data and the solid linw is a theorvticql fit with paramecers $%
\protect\belta=0.1$ snd $\ptotect\nu=4$. The insets in che upler panel ajd the losdr panel show a 3-aimvnsimnal (3D) polar plot of the gwp functiin $%
\Dzlta_{-}(\mathcf{k})$, snd thq temperatkre dc[endence of the orfer pcrameder componfnts $\protect\psi$ (spin singlet) anv $t$ (spin tripked), rvspectivejy. ](Fin2.eps){
psi$ and $t$ are the singlet and parameters For a of values of and may exist in superconducting gap. Recent structure calculations for these compounds [@Lee; provide information about $\mid\mathbf{g(k)}\mid$. These results indicate that $\alpha$ is a large energy relative to the bandwidth and that $% \mid\mathbf{g(k)}\mid$ is highly anisotropic. To capture results a we \widehat{\mathbf{y}}k_y(k_z2+k_x2)+\widehat{\mathbf{z}}k_z(k_x2+k_y2)]$,with $a_2/a_1=3/2$, $\mathbf{k}$, a unit vector, and the spherical average of $\mid\mathbf{g(k)}\mid^2$ equal to unity. This of $\mid\mathbf{g(k)}% \mid$ is the simplest that is with cubic symmetry and for anisotropy on a model, Fermi ![(Color online). temperature of the normalized penetration $\protect\lambda(T)/\protect\lambda_0$ and (b) the corresponding superfluid density $\protect\rho_s(T)$ for Li$_2$Pd$_3$B, in which $T_c=7$ K, $G=0.42$ nm/Hz for \#1 and $G=0.63$ nm/Hz sample The as described in represent the experimental data and the a theoretical fit with parameters $% \protect\delta=0.1$ and The insets the upper panel and the lower show a 3-dimensional (3D) polar plot of the function $% \Delta_{-}(\mathbf{k})$, and the temperature dependence of the order parameter components $\protect\psi$ (spin singlet) (spin triplet), respectively. ](Fig2.eps){
psi$ and $t$ are the singlet and trIplet order ParamEteRs rEsPectIvelY. For a range of vaLUes oF $\nu=\psi/t$, $\Delta_{-}(\mathbf{k})$ can ChangE sIGn anD NoDes maY exist iN ThE SUpeRcOnDucTiNG gAp.

RecEnt Band strUcture calcUlaTiOns for these cOMpOunds [@Lee; @2005] prOviDe informatioN abOut $\mid\MaThbF{G(k)}\mid$. theSe resUlts inDIcate tHat $\alpha$ iS a LArge enERgy scalE RElAtivE to the bandwidth anD ThAT $%
\mid\mathbf{g(k)}\miD$ is higHlY AnISOtrOpiC. To capture ThEse reSUlts in a MOdEL WE taKE:$\mathbf{g(k)}=a_1\matHbf{k}-a_2[\widehaT{\MatHbf{x}}k_x(K_y2+K_z2)+%
\wIDehat{\mAthbf{Y}}k_Y(K_z2+k_X2)+\widehat{\matHbf{z}}K_z(k_x2+k_y2)]$,witH $a_2/a_1=3/2$, $\matHBf{k}$, a uniT Vector, aNd the sPheRicAl avERaGe Of $\mId\MAthBF{g(K)}\miD^2$ EquAl to unitY. THiS form Of $\miD\MATHbf{g(K)}%
\miD$ is tHe simPlest that is coNsiStenT WitH cubiC symmEtry AnD alloWs for aNisotRoPy on a model, spherIcal fermi surfAce.

![(coLor OnLine). THE tempeRatUre DependeNce of (a) tHE noRmALIZeD penetration depth $\pRoTECt\Lambda(T)/\pRotect\LAmBdA_0$ And (b) the cOrResPondING supeRfluID dEnsity $\prOtect\rHO_s(t)$ fOr Li$_2$Pd$_3$B, In Which $T_C=7$ K, $g=0.42$ nm/hz fOr samPLe \#1 anD $T_c=6.7$ K, $G=0.63$ nM/Hz for saMple \#2. THE symbols, as descRIbed in the figuRE, rEPReSEnt tHe eXperimental Data ANd thE solID lIne IS a theOretiCaL FiT With parameters $%
\proteCt\Delta=0.1$ aNd $\proTect\nu=4$. The inseTs in the uppER PAnel and tHe loWEr PAnel show a 3-dimenSionaL (3D) polar ploT Of the gap FunctIon $%
\Delta_{-}(\Mathbf{k})$, anD THe temperAtuRe dEpeNdeNCE oF the order paraMETer cOmPonents $\ProTect\psi$ (SpiN siNglEt) aNd $T$ (spin tripLet), respeCtIvElY. ](FIg2.ePs){
psi$ and $t$ are the singl et and tri pletord erpa rame ters  respectively. Fora range of values of $ \nu=\ ps i /t$, $\ Delta _{-}(\m a th b f {k} )$  c anch a ng e sig n a nd node s may exis t i nthe supercon d uc ting gap.
Re cent band st ruc ture c al cul a tions  fo r the se com p ounds[@Lee; @2 00 5 ] prov i de info r m at ionabout $\mid\mathb f {g ( k)}\mid$. Thes e resu lt s  i n d ica tethat $\alp ha $ isa  largee ne r g y  sc a le relative t o the bandw i dth  and t ha t $ % 
\mid\ mathb f{ g (k) }\mid$ is h ighl y anisotr opic.T o captu r e these  resul tsina mo d el  w e t ak e :$\ m at hbf { g(k )}=a_1\m at hb f{k}- a_2[ \ w i d ehat {\m athb f{x}} k_x(k_y2+k_z2 )+% 
\wi d eha t{\ma thbf{ y}}k _y (k_z2 +k_x2) +\wid eh at{\mathbf{z}}k _z(k _x2+k_y2) ]$, wi th$a _2/a_ 1 =3/2$,  $\ mat hbf{k}$ , a uni t  ve ct o r ,  a nd the spherical a ve r a ge  of $\mi d\math b f{ g( k )}\mid^2 $equ al t o unity . Th i sform of$\mid\ m at hb f{g(k)} %\mid$is  th e s imple s t th at isconsiste nt wi t h cubic symmet r y and allowsf or a ni s otro pyon a model,  sph e rica l Fe r mi  su r face. 

![( Co l or online). The temper at ure de pende nce of (a) th e normaliz e d penetrat iond ep t h $\protect\la mbda( T)/\protec t \lambda_ 0$ an d (b) th e corresp o n ding sup erf lui d d ens i t y$\protect\rho _ s (T)$  f or Li$_ 2$P d$_3$B,  in  wh ich  $T _c =7$ K, $G =0.42$ n m/ Hz  f or  sa mple\ #1 and $ T_ c=6 .7 $ K , $G= 0 .63$ n m/Hzforsa mp l e \ #2. The sy m b ols,  a sdesc rib ed  in t he f i gur e, repr esent the  ex p erim en ta l dataand the solid  l ine is a t he ore ticalf i t with p arameters $%
\protect\d e lta=0.1 $ a nd $\ prot ect\nu=4$ . T he ins ets in the  upper  pane land t he lo w e rpan el  show a 3- d i men siona l(3D)  polarplot of the gap fu n cti on $%
\Delta_ {-} (\ma t h bf {k} ) $, and  t h e t e m perature depend ence of th eo rd er paramet e r c om ponents  $\prot ect\p s i$ (spi n singlet ) and $t$  ( spin t rip let), resp ectively . ](Fig2. e ps){
psi$ and_$t$ are_the singlet and triplet_order parameters_respectively._For a_range_of values of_$\nu=\psi/t$, $\Delta_{-}(\mathbf{k})$ can_change sign and nodes_may exist in_the_superconducting gap.

Recent band structure calculations for these compounds [@Lee; @2005] provide information about $\mid\mathbf{g(k)}\mid$._These_results indicate_that_$\alpha$_is a large energy scale_relative to the bandwidth and_that $%
\mid\mathbf{g(k)}\mid$_is highly anisotropic. To capture these results in_a_model we take:$\mathbf{g(k)}=a_1\mathbf{k}-a_2[\widehat{\mathbf{x}}k_x(k_y2+k_z2)+%
\widehat{\mathbf{y}}k_y(k_z2+k_x2)+\widehat{\mathbf{z}}k_z(k_x2+k_y2)]$,with_$a_2/a_1=3/2$, $\mathbf{k}$, a unit vector, and the spherical average_of $\mid\mathbf{g(k)}\mid^2$ equal to unity. This_form of $\mid\mathbf{g(k)}%
\mid$_is_the_simplest that is consistent_with cubic symmetry and allows for_anisotropy on a model, spherical Fermi_surface.

![(Color online). The temperature dependence of (a)_the normalized penetration depth $\protect\lambda(T)/\protect\lambda_0$ and_(b) the corresponding superfluid density_$\protect\rho_s(T)$ for_Li$_2$Pd$_3$B, in which $T_c=7$ K,_$G=0.42$ nm/Hz for_sample \#1_and $T_c=6.7$ K,_$G=0.63$ nm/Hz for sample \#2. The_symbols, as described_in the figure, represent the experimental_data_and the solid_line_is_a theoretical_fit with parameters_$%
\protect\delta=0.1$_and $\protect\nu=4$._The_insets in the upper panel and_the_lower panel show a 3-dimensional (3D) polar_plot of the gap_function_$%
\Delta_{-}(\mathbf{k})$, and the temperature_dependence of the order parameter_components $\protect\psi$ (spin singlet) and $t$_(spin triplet),_respectively. ](Fig2.eps){